Thermal/Mechanical Durability of Polymer-Matrix T. S., K.S. Whitley, R.W. Grenoble, T. Bandorawalla,...
Embed Size (px)
Transcript of Thermal/Mechanical Durability of Polymer-Matrix T. S., K.S. Whitley, R.W. Grenoble, T. Bandorawalla,...
Gates, T. S., K.S. Whitley, R.W. Grenoble, T. Bandorawalla, Thermal/Mechanical Durability of Polymer Matrix Composites in Cryogenic Environments, AIAA-2003-7408, 44th Annual AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference, Norfolk, VA, April 7-10, 2003.
Thermal/Mechanical Durability of Polymer-Matrix Composites in Cryogenic Environments1
Thomas S. Gates*, Karen S. Whitley, Ray W. Grenoble , Tozer Bandorawalla
NASA Langley Research Center Hampton, VA 23681
Introduction Abstract The National Aeronautics and Space
Administration (NASA) Space Shuttle is the only launch vehicle in service today with reusable components. To address the issues of an aging Space Shuttle fleet, and to advance key technologies associated with increased performance, NASA has initiated the Space Launch Initiative (SLI) program. One of the key performance advances identified for next-generation reusable launch vehicles (RLVs) is the reduction in structural weight through the use of advanced materials and manufacturing methods. This reduction in structural weight must be tempered against the safety and reliability criteria associated with damage tolerance, and lifetime durability.
In order to increase the reliability of the next generation of space transportation systems, the mechanical behavior of polymeric-matrix composite (PMC) materials at cryogenic temperatures must be investigated. This paper presents experimental data on the residual mechanical properties of a carbon fiber polymeric composite, IM7/PETI-5 as a function of temperature and aging. Tension modulus and strength were measured at room temperature, 196C, and 269C on five different specimens ply lay-ups. Specimens were preconditioned with one set of coupons being isothermally aged for 576 hours at 184oC, in an unloaded state. Another set of corresponding coupons were mounted in constant strain fixtures such that a constant uniaxial strain was applied to the specimens for 576 hours at 184oC. A third set was mechanically cycled in tension at 184oC. The measured properties indicated that temperature, aging, and loading mode can all have significant influence on performance. Moreover, this influence is a strong function of laminate stacking sequence. Thermal-stress calculations based on lamination theory predicted that the transverse tensile ply stresses could be quite high for cryogenic test temperatures. Microscopic examination of the surface morphology showed evidence of degradation along the exposed edges of the material because of aging at cryogenic temperatures.
It is envisioned that the next-generation RLV will have integral liquid-hydrogen (LH2) and liquid-oxygen (LOX) cryogenic fuel tanks that not only function to contain the fuel but must also perform as load-carrying structure during launch and flight operations. Presently, is appears that replacement of traditional metallic cryogenic fuel tanks with polymeric matrix composite (PMC) tanks may lead to significant weight reduction and hence increased load-carrying capabilities.
Despite the lack of long-term flight data, there is some history of design and testing of PMC cryogenic tanks that includes the National Aerospace Plane (NASP)1, DCX-A2, X-333, and other launch vehicle applications4,5. These programs have considered several tank wall design concepts including externally stiffened shells of PMC material or thin-walled sandwich shells constructed with a lightweight core and PMC facesheets.
________________ *Senior Materials Research Engineer, Mechanics and Durability Branch. Associate Fellow, AIAA. Aerospace Engineer, Mechanics and Durability Branch. Graduate Co-op, Mechanics and Durability Branch. Post-doctoral associate, Old Dominion University.
1 Copyright 2003 by the American Institute of Aeronautics and Astronautics, Inc. No copyright is asserted in the United States under Title 17, U.S. Code. The U.S. Government has a royalty-free license to exercise all rights under the copyright claimed herein for Government Purposes. All other rights are reserved by the copyright owner.
Regardless of the design, the next generation of PMC-based tanks will be required to safely carry pressure and flight loads and to operate over temperatures that may range from 250oC to +120oC. From a durability perspective, the primary performance criteria of the PMC material is to retain mechanical properties within allowable limits over the life-time of the tank while minimizing loss of cryogenic fuel because of permeation or leakage through the tank wall.
Other than space launch vehicle applications, there have been very few uses of PMCs as structural
1 American Institute of Aeronautics and Astronautics
materials in cryogenic environments and consequently the available literature provides limited experimental data on the mechanical properties of polymers or PMCs operating at cryogenic temperatures.
Related to durability, long-term fatigue tests were performed by Pannkoke6 on unidirectional thermoplastic composites at 196oC. The fatigue strength was found to be only 60% of the static strength at 106 cycles. In this work, it was recognized that large thermal stresses degraded the fatigue performance. In a series of articles by Alhborn7,8, static and cyclic thermal/mechanical tests were performed on unidirectional and cross-ply thermoplastic composites. He conducted isothermal tests at 23oC, 196oC, and 269oC and cyclic thermal tests between 196oC and 23oC. Strength, damage, and fatigue life were measured for all test conditions. It was found that the effects of temperature on static strength were largely related to the matrix-dominated properties, shear and transverse tension. Increases in matrix-dominated strength as the temperature is decreased could be offset by the development of thermal-stress-induced cracks. As in previous studies, the fatigue life was reduced as the test temperature was decreased. Matrix dominated properties are a function of the polymer material properties. For amorphous and crystalline polymeric materials, Perepechko9 provides details on a number of non-mechanical properties including thermal expansion, thermal conductivity, as well as viscoelastic or dynamical mechanical properties. From these studies, it is clear that many of the cryogenic polymer properties are not linear with respect to temperature.
Schutz10 has provided a compilation of test data for several PMC material systems. He showed that, in general, static properties such as tensile modulus, tensile strength, and compressive strength all increased as the test temperature was decreased from 23oC to 269oC. Once again, it was found that thermal stresses had a large influence on behavior and that the sensitivity of matrix-dominated properties to temperature can be used to help explain the stress-strain response of laminated composites.
Of these matrix-dominated properties, transverse ply strength may play a critical role in the development and growth of residual-stress-induced matrix cracks. The range of thermal and mechanical loading over which steady-state matrix cracking may occur was investigated recently by Schoeppner11. Additional studies related to matrix crack development in PMCs because of cryogenic temperature exposure is found in ref.12 and ref.13.
The lack of long-term thermal/mechanical performance data on an advanced composite, such as IM7/PETI-5, subjected to a cryogenic environment, is clearly evident. Therefore, the objectives of the present paper are to assess the thermal/mechanical durability of
IM7/PETI-5 at cryogenic temperatures, document the test methods, and provide insights into the effects of temperature and aging on mechanical performance. The selected test conditions represent a range of exposure times, loads and temperatures similar to those experienced during the lifetime of a cryogenic, hydrogen fuel tank. Results are given for tension and compression-loaded coupons subjected to temperatures that ranged from room temperature to 269C. Fundamental, lamina-level material properties were measured, analyzed, and correlated against test environment. Residual stiffness and strength, and damage will be given as a function of both cryogenic test temperatures and pre-test cryogenic aging conditions. Results from thermal stress analysis are presented to illustrate the effect of temperature and aging on the stress state in typical laminates.
It is recognized that a broad spectrum of factors influence the properties of PMCs including material selection, composite fabrication and handling, aging or preconditioning, specimen preparation, laminate ply lay-up, test procedures, etc. This study focuses on test temperature, preconditioning methods (load, temperature and time), and laminate configuration as the primary test variables. It is expected that the results of this study will be important in the development of future material qualification methods and design verification testing.
The PMC material used in this study, IM7/PETI-5, consisted of a continuous, high-strength, intermediate-modulus, carbon fiber in a thermoplastic polyimide matrix. All test materials were laminated composites, fabricated at the NASA Langley Research Center. These composite panels consisted of unidirectional and angle-ply laminates, (12, 12, 3S, 3S), and a 13-ply quasi-orthotropic laminate ([45/903/-45/ 0 3]S). The bar notation over the 0 indicates that the 03 ply group is not symmetric. Fig. 1 provides a schematic illustrating the coordinate system for the fiber orientations relative to the specimen dimensions.
These lay-ups were chosen to provide basic lamina-level material constants and in the case of the